Z. Rebaoui, W. Bachir Bouiajra, M. Abboun Abid, A. Saidane, D. Jam-mel, M. Henini, J.F. Felix

PII: S0167-9317(17)30017-5 DOI: doi:10.1016/j.mee.2017.01.010

Reference: MEE 10437

To appear in:

Received date: 9 June 2016 Revised date: 3 January 2017 Accepted date: 11 January 2017

Please cite this article as: Z. Rebaoui, W. Bachir Bouiajra, M. Abboun Abid, A. Saidane, D. Jammel, M. Henini, J.F. Felix, SiC polytypes and doping nature eﬀects on electrical properties of ZnO-SiC Schottky diodes, (2017), doi:10.1016/j.mee.2017.01.010

## ACCEPTED MANUSCRIPT

SiC polytypes and doping nature effects on electrical properties of ZnO-SiC Schottky diodes Z. Rebaouia, W. Bachir Bouiajraa, M. Abboun Abida, A. Saidanea, D.Jammelb, M. Heninib, J.F.Felixc

a

CaSiCCE Laboratory, ENP-Oran, B.P 1523 El M'Naouar, Oran 31000, Algeria

b

School of physics and Astronomy, Nottingham University , NG72RD, United Kingdom.

c

Universidade de Brasília, Instituto de Física, Núcleo de Física Aplicada, Brasília, DF70910-900, Brazil . zoheirmed@yahoo_fr.

Abstract

Electrical properties of ZnO/SiC Schottky diodes with two SiC polytypes and N and P doping are investigated. Characterization was performed through I–V and C–V–f measurements. Schottky barrier height (Φb), ideality factor (n), and series resistance (Rs) were extracted from forward I–V characteristics.

(Φb), carrier’s concentrations (Nd-Na) and (Rs) frequency dependence were extracted from C–V–f

characteristics. The extracted n values suggest that current transport is dominated by interface generation-recombination and/or barrier tunneling mechanisms. When changing SiC polytypes, the rectifying ratio of ZnO/n-4HSiC is found to be twice that of ZnO/n-6HSiC. A change in doping nature gave a leakage current ratio of 40 between ZnO/p-4HSiC and ZnO/n- 4HSiC. These results indicate that ZnO/p-4HSiC diodes have a complex current transport compared to diodes on n-type SiC. From I-V measurements, barrier height values are 0.63eV, 0.65eV and 0.71 eV for heterojunction grown on n-6HSiC, n-4HSiC and p-4HSiC, respectively. C-V measurements gave higher values indicating the importance of interface density of states. Nss values at 1MHz frequency are 4.54×10

11

eV-1 cm-2, 3×1012 eV-1 cm-2 and 8.13×1010 eV-1 cm-2 for ZnO/n-6HSiC, ZnO/n-4HSiC and ZnO/p-4HSiC, respectively. Results indicate the importance of SiC polytypes and its doping nature.

Keywords: ZnO/SiC; SiC polytypes; I–V characteristics; C–V-f measurements; Electrical properties.

1. Introduction

Silicon Carbide (SiC) is a promising semiconductor material for electronic power applications. Among its properties, there are its high electric field strength, high electron drift velocity, high thermal conductivity, radiation and harsh ambient endurance, high melting point that lead to significant advantages for power switching devices. It grows in many different polytypes, but the most studied are the 3C, 4H, and 6H SiC [1,2]. On the other hand, ZnO has a direct wide band gap (3.37 eV), large exciton binding energy and piezoelectric properties. These properties make ZnO a strong candidate for applications in solar cell development, photodiodes, and surface acoustic wave devices and so on [3,4].

To date, little has been done on this combination of materials. SiC is a good candidate for use as substrate for ZnO nanostructure growth in many applications. SiC and ZnO have the same wurtzite crystal

symmetry and relatively small lattice mismatch (

###

5%) [5]. Ataev et al. [6] were the first to report on the fabrication of ZnO/p-6HSiC heterostructures by chemical vapor deposition, which presented poorcurrent–voltage characteristics. A decade ago, Alivov et al. [7, 8] reported on the growth of ZnO/p-6HSiC heterostructures diodes by plasma-assisted molecular-beam epitaxy (MBE). In the same time, Yuen et al. [9] demonstrated the possibility to fabricate ZnO: Al/p-4HSiC heterojunction light-emitting diodes (LEDs) by a filtered cathodic vacuum arc technique. More recently, Y.T. Shih et al. [10] used atomic layer deposition to fabricate ZnO/p-4HSiC and n–ZnO/i–ZnO/p-4HSiC heterojunction LEDs.

A number of process methodologies have been developed for the fabrication of reproducible high quality Schottky contacts with SiC nanostructures, but controversies remain with regard to Schottky barrier height and ideality factor of SiC Schottky contacts [11,13]. Deviations in barrier heights and ideality factor have been attributed to effects of asymmetric contacts and influence of interfacial layers and/or surface states [14,15]. Schottky barrier height depends not only on work function of metal but also on pinning of Fermi level by surface states, image force lowering of barrier, ﬁeld penetration and existence of an interfacial insulating layer. These effects change absolute current value at low bias values by lowering Schottky barrier [18].

## ACCEPTED MANUSCRIPT

This paper reports on the effects of polytypes and doping nature on electrical properties of ZnO/ n-6HSiC, ZnO/n-4HSiC and ZnO/p-4HSiC based Schottky diodes. Various measurements such as current-voltage (I-V), capacitance-voltage-frequency (C-V-f) and conductance-frequency (Gp/

###

) are used. Parameters studied are ideality factor (n), series resistance (Rs), barrier height (###

*) and interface states density (Nss).*

_{b}These were calculated using Cheung, Lien and Hill-Coleman [19] methods. 2. Sample details

All fabrication steps [20] were done in clean room (class 1000) using metal-oxide-semiconductor (MOS) grade chemicals. 4H-SiC and 6H-SiC wafers (Si terminated) were provided by Cree Research

Corporation. In both cases, the epitaxial layer had a doping of 5x1015cm-3 and its thickness was 4.9 µm. The epitaxial layer was grown 8°9 off-axes for 4HSiC and 3°22 off-axes for 6HSiC. Total wafer

thickness was 421 µm for 4HSiC and 382 µm for 6HSiC. After cleaning of substrates by a modified RCA process, a large area backside electrical contact was obtained by thermal evaporation of 99.9% pure Al (thickness of 200 nm) and Ni (thickness of 50 nm), respectively. These electrical contacts were deposited by vacuum thermal evaporation at a base pressure below 10−6 Torr using a BOC Edwards 306 system. After evaporation, the contacts were annealed in vacuum for 5 min, at 900°C to form Ohmic contact to bottom of SiC bulk substrate [21, 22]. These SiC substrates with backside electrical contact were loaded in a thermal evaporator for evaporation of 99.99% ZnO powder through a metal mask. A 120 nm thick ZnO disc was deposited onto SiC epitaxial layer. Fig.1 shows a schematic diagram of Ni/Al/SiC/ZnO heterojunction diode structure including layer thicknesses. Schottky contacts were formed at ZnO/SiC doped epilayer [23, 24].

Current-voltage (I–V) measurements were carried out using an Agilent precision semiconductor parameters analyzer (4156C). The capacitance–voltage–frequency (C-V-f) and conductance –voltage– frequency (G-V-f) measurements were carried out with an Agilent LCR meter (4980A).

3. Current-voltage measurements

After fabrication of Schottky diodes, first step is to measure their current-voltage (I-V) characteristics that provide immediate information about quality and suitability of diodes. I-V curves may be described by thermionic emission model, with a series resistance Rs [25], according to equation (1).

( )

exp(*q V* *IRs* ) 1

*I* *Is*

*nkT*

_{} _{}

_{ }(1)

Where q is electronic charge, V is applied voltage, k is Boltzmann constant, (n) is ideality factor, (Is) is saturation current, and (T) is absolute temperature in Kelvin. The values of (n) and (Is) are determined from experimental data. Saturation Current (Is) is given by:

** 2_{exp(} *B*_{)}
*s*

*q*

*I* *AA T*

*kT*

(2)

Where

###

*is barrier height, A is diode area and A** is Richardson’s constant theoretically taken as*

_{B}2 *

** 2 2

2

4

32

*qk m*

*A* *Acm K*

*h*

###

(m*=0.28m0

,

for ZnO and A=0.0314cm2) [26].

Typical I-V characteristics of Schottky diodes are shown in Fig.2. On Fig.2.a, one observes that ZnO/n-4HSiC can pass more current than ZnO/n-6HSiC. This is attributed to its higher vertical a-axis electron mobility [27]. On the other hand, forward bias behavior of I–V characteristics of these devices is approximately similar for both SiC polytypes. Exponential behavior of current at low forward voltages indicates a thermionic emission current transport behavior. This exponential dependency at lower voltages range can be attributed to a depletion region formation between ZnO and SiC [28].

## ACCEPTED MANUSCRIPT

0( ) exp(*qVd*) 1 exp( *qVd*)

*J V* *J*

*nkT* *kT*

_{} _{}

(3)

Where J0 is the saturation current density given by:

** 2

0 exp( )
*b*
*q*

*J* *A T*

*kT*

(4)

J0 is deduced from the straight line intercept of Ln (J)-V curve. Ideality factor (n) of Schottky barrier is an

important parameter that indicates perfection of metal-semiconductor junction. It is determined from slope of semi log J-V characteristics in exponential region and given by:

(ln )

*dV*
*n*

*d* *J*

With *q*

*kT*

(5)

Barrier height is an electrostatic barrier to charge transfer across metal/semiconductor interface.

###

*can be written as:*

_{b}** 2
1
ln( )
*b*
*o*
*A T*
*J*

(6)

When *V* 3*kT q*/ , equation (3) becomes:

** 2

exp( *q* *B*) exp(*qV* )

*J* *A T*

*kT* *nkT*

(7)

There are four mechanisms that contribute to current transport across a metal -semiconductor interface: (i) thermionic emission over potential barrier, (ii)quantum-mechanical tunneling of carriers through potential barrier, (iii) carrier recombination in depletion region and (iv) carrier recombination in neutral region of semiconductor [31]. For wide band gap semiconductor materials such as SiC, the dominant contribution to current transport comes from thermionic emission (TE) of electron over barrier and tunneling of electrons through the barrier. If SiC material of Schottky contacts is not heavily doped and the operating temperature is not very low, thermionic emission (TE) term will be dominant. The tunneling term will only be significant if SiC is heavily doped or the device is operating under low temperature or is blocking high reverse voltage. Carrier recombination in depletion region may dominate in case of a higher density of states at the metal-semiconductor interface.

LnJ-V characteristics of Fig.3.a show a difference in rectifying behavior between n-4HSiC and n-6HSiC heterojunctions. From insight of Fig.3.a, ZnO/n-4HSiC calculated rectifying ratio (forward to reverse current ratio, IF/IR) is found to be twice that of ZnO/n-6HSiC. Reverse current density is about 1.39*10-5

A/cm2 for ZnO/n-4HSiC and 6.74*10-5 A/cm2 for ZnO/n-6HSiC. Devices exhibited very good

rectification ratio, substantially low leakage current and indicate formation of rectifying behavior between ZnO and n-type SiC with a noticeable superiority for 4HSiC substrates. These values are better than values previously reported, where more sophisticated and expensive techniques were used [6,9].

In Fig.3.b, ln J–V characteristics show doping nature effects on Schottky diodes. P type characteristics are different from those of N type. At a reverse bias of -5 V, leakage current ratio between ZnO/p-4HSiC and ZnO/n-4HSiC is 40. Calculated saturation current for ZnO/n -4HSiC is 9.663x10-7 A/cm2 and for ZnO/p -4HSiC is 9.384x10-8 A/cm2 giving a ratio of 10.Among these two heterostructures, the one on p-4HSiC substrate has a higher leakage current .These results indicate that heavy doping of p-4HSiC makes tunneling current more probable [32]. Heterojunction diodes fabricated from ZnO grown on n-4HSiC exhibited more stable rectification characteristics and higher IF/IR value.

Fig.3.b inset shows forward current of Schottky diodes that tends to saturate at bias voltages above 0.7V and 1.25V for N type and P type, respectively. This relatively low forward current in P type is attributed to higher series resistance. A high value of series resistance reduces mobility of electrons and holes. Cheung method [33] was applied to evaluate series resistance Rs and ideality factor n using a modified

equation (7):

/

(ln ) *s*

*dV* _{R AJ}_{nkT q}

*d* *J* (8)

** 2

( ) ( / ) ln(J/ (A ))

*H J* *V* *n kT q* *T* (9)

With *H J*( )*R AJ _{s}*

*n*

*(10)*

_{B}## ACCEPTED MANUSCRIPT

intercept and slope of dV/d(lnJ) versus J plots. These values are shown in table 1. A plot of H(J) versus J
will also lead to a straight line with y-axis intercept equal to *n*

###

*. Substitution using deduced n value into Equation (10) gives*

_{b}###

*. Slope of H(J) versus J determines RS that can be compared with value obtained*

_{b}from dV/d(lnJ) versus J.

The ideality factor, as estimated from equation (1), was found to be >4 suggesting that the mechanism of transport is not thermionic emission only. Other mechanisms of current transport such as generation - recombination in space charge region and/or barrier tunneling [34, 35] exist. All these forms of current can be interface defects assisted. n values were found to be 6.32, 6.70, and 4.67 for ZnO deposited respectively on n-6HSiC, n-4HSiC and p-4HSiC; in good agreement with results reported by Felix et al.[11].

SiC polytypes affect ideality factor with that of ZnO/n-6HSiC smaller than that of ZnO/n-4HSiC. This difference can be ascribed to interface dipoles or speciﬁc interface structures. Defects induced during elaboration at interface ZnO/substrate are known to result from reactions between the metal and carbon face of SiC crystal [36].

Calculated barrier height values are 0.63eV, 0.65eV and 0.71 eV for heterojunctions grown on n-6HSiC, n-4HSiC and p-4HSiC, respectively. The small difference in barrier high value between devices with different polytypes can be attributed to difference in band gap between 6H-SiC and 4H-SiC substrate which is about 3 eV and 3.2eV, respectively [28].

Doping nature has an effect on barrier height, which decreases from 0.71eV to 0.65 eV when passing from P type to N type Schottky diodes. Electron tunneling traps localized in interfacial layer close to p-4HSiC surface are known to increase

###

*. Increase in ideality factor from 4.67 to 6.70 is also associated with surface states and/or carrier generation transport near interface [11].*

_{b}Series resistance is a very important parameter in Schottky diodes. It is the sum of contact resistance and semiconductor device resistance in direction of current flow. A plot of dV/dLn (J) versus J is linear and from slope we deduce values of series resistance. Rs values obtained for ZnO grown on 6HSiC,

n-4HSiC and p-n-4HSiC, are 205.5Ω, 15.50Ω and 12.8KΩ respectively. These values are lower than those reported by Felix et al. [11]. Series resistance can also be determined from H(J) versus J plots, Fig. 4. For ZnO deposited on n-6HSiC, n-4HSiC and p-4HSiC, series resistance of devices are respectively 218.5Ω, 14.5Ω and 14.8KΩ. These values of Rs are in good agreement with those obtained from dV/dLn (J) versus

J plots. Rs for P type is higher than N type because barrier to holes injection is higher compared to that of

electrons. ZnO/n-6HSiC had a higher Rs than ZnO/n-4HSiC devices. This can be attributed to carriers’

removal effect, mobility change and/or reduction in free carriers’ concentrations [37, 33]. 4. Capacitance-voltage Measurements

Plotting inverse squared junction capacitance against applied reverse voltage of ZnO/SiC Schottky

contacts is used to find built in potential (Vbi), barrier height (φb0) and carrier concentration (ND), equation

(11) and Fig.5.

2 2

1 _{2(} _{) / (} _{)}

*bi* *D*

*V* *V* *A qN*

*C* (11)

ND is deduced from slope and Vbi from intercept.

2 2

2 / ( ) 1/ ( (1/ ) / )

*D* *s*

*N* *q A* _{} *d* *C* *dV* _{} (12)

Where

###

*9*

_{s}###

_{0}is permittivity [38], A is Schottky contact area, Vbi is built in potential, and ND is carrier

concentration. NC=2(2πm*kT/h 2

)3/2=4.8x1018cm-3 is conduction band density of states at T =300 K. V0,

x-intercept, is related to build in potential Vbi by: 0 /

*bi*

*V* *V* *kT q* (13)

Barrier height

###

_{b}_{0}is given by:

0 / ln( / )

*b* *Vbi* *kT q* *NC* *ND*

(14)

Density of states in conduction band edge is given by:

3 3 2

2((2 * ) /

*C*

*N* *m kT* *h* (15)

## ACCEPTED MANUSCRIPT

Carriers concentrations and

###

_{b}_{0}were calculated from above equations and are shown in Table 2. Capacitance–voltage measurements were made at high frequency (1 MHz) to reduce interface state charges contribution to capacitance. There is a difference between barrier height values extracted from J– V and C–V measurements inTable1 and Table 2, respectively.

Barrier height obtained from C–Vmeasurements is comparatively larger than barrier heights obtained from J–Vmeasurements. Difference is attributed to interface effects [39,40]. Indeed, current in J–V measurement is dominated by current flowing through low barrier height region. In C–V measurements, barrier height is influenced by distribution of charge at depletion region boundary. This charge

distribution follows weighted arithmetic average of barrier height inhomogeneity. Hence, capacitance is insensitive to potential fluctuations on a length scale of less than space-charge width and therefore C–V method averages over whole area [40].

Slope of (1/C2) versus V gives carrier concentration (Nd-Na), while intercept gives built-in potential (Vbi).

Values of Vbi and Nd are 0.825 V and 0.53x10 +15

(cm-3) for ZnO/n-6HSiC, and 1.05V and 0.50x10+15(cm-3) for ZnO/n-4HSiC. For ZnO/p-4HSiC, Vbi and Na are 0. 675V and 23.4x10

+15

(cm-3), respectively. These Nd and Na values are in good agreement with data provided for SiC substrate.

Difference in barrier heights between ZnO/n-6HSiC and ZnO/n-4HSiC is about 0.22 eV, which corresponds to difference between their respective band gaps. Barrier height is generally higher for ZnO/n-4HSiC than for ZnO/n-6HSiC, due to interface state density. Barrier height is found to be around 0.9372 eV for ZnO/n-6HSiC and 1.1638 eV, For ZnO/n-4HSiC respectively, indicating a strong Fermi-level pinning for ZnO/n-6HSiC. Interface states density was estimated to be of 4.54*1011eV-1cm-2 for ZnO/n-6HSiC. Barrier height of N type Schottky diodes was twice higher than P type. This is attributed to big difference in surface states densities.

Other effects that may be affecting Schottky barrier height can be revealed by studying forward capacitance–voltage and conductance–voltage as function of frequency (from 1 MHz to 10 kHz). Fig.6 shows C–V–f characteristics of ZnO/n-6HSiC, ZnO/n- 4HSiC and ZnO/p-4HSiC Schottky diodes. Diode capacitance is quasi-independent of frequency at low voltages up to 0.5 V for N type 6HSiC and 0.25 V for 4HSiC.

Measured capacitance of Schottky diodes changed with bias voltage and frequency. Such dependency is related to Schottky barrier heights, impurity levels and high series resistances.

Capacitance value decreases with increasing frequency for all structures. It exhibits a peak at positive voltage for N type SiC and at negative voltage for P type SiC. This peak has been related to interface states in band gap and series resistance [41]. Capacitance peaks changed with an increase in interface state density occupancy that is more and more activated when decreasing frequency. Series resistance can also affect the height of peak capacitance [42].

From Fig.6 , one can see that the doping effect has lead to a 5 times higher peak for N type SiC than P type SiC, while a difference in polytypes has lead to a 2 times higher peak for 4HSiC than 6HSiC. These results reflect differences in interface states densities or traps densities between ZnO/n- 4HSiC, ZnO/p- 4HSiC and ZnO/n-6HSiC Schottky diodes.

Fig.7 shows measured G/ω–V characteristics of ZnO/SiC Schottky diodes, measured at various frequencies at room temperature.

One can see that conductance of Schottky diode ZnO/n-6HSiC, ZnO/n-4HSiC is different from that of ZnO/p-4HSiC. As expected, conductance increases with increasing positive voltage for ZnO/n-type SiC and with increasing negative voltage for ZnO/p-type SiC. It decreases with increasing frequency in all cases due to increasing deactivation of interface states responsible for capture and emission of carriers. To show dependence of interface states density on frequency, Hill–Coleman [19] used:

2 2

max max

2 / ( )( * _{m}*/ ) / ((

*/ ) /*

_{m}*) (1*

_{ox}*/*

_{m}*)*

_{ox}*Nss* *qA G*

###

*G*

###

*C*

*C*

*C*(16)

Where A is contact area of diode,

###

is angular frequency, Cm and (Gm/###

) max are maximum measuredcapacitance and conductance and Cox is native insulator layer capacitance given by [43, 45]:

2 0

1 ( *m* ) *i*

*ox* *m*
*m*
*A*
*G*
*C* *C*
*C*

###

###

###

_{}

_{}

(17)

## ACCEPTED MANUSCRIPT

Fig.8. shows density of interface states versus frequency. *Nss *values for ZnO/n-6HSiC are lower than

ZnO/n-4HSiC. Such behavior can be ascribed to a thicker oxide layer at ZnO/n-6HSiC interface than at ZnO/n-4HSiC interface. This is due to a difference in interface dangling bonds between 6HSiC and 4HSiC surfaces.

*Nss *values for ZnO/p-4HSiC are lower than ZnO/n-4HSiC. Since interface states play a very important

role in current flow mechanism in electronic devices, one may conclude that carrier’s recombination will
be important in ZnO/n-4HSiC leading to I-V characteristics dominated by recombination. This is in good
agreement with calculated n values. High *Nss* values are known to affect series resistance [46]. To show

this effect, series resistance Rs is being plotted using maximum measured values of capacitance Cm and

conductance Gm [43,41] according to:

2 2 2

### / (

### )

*Rs*

###

*Gm*

*Gm*

###

###

*Cm*

(18)
Fig.9 shows series resistance changes with frequency for ZnO/6HSiC, ZnO/ n-4HSiC and ZnO/p-4HSiC Schottky diodes. For N type devices, series resistance peak decreases with higher frequencies and slightly shifts with greater voltages. Opposite behavior is seen to happen for P type devices. Since series

resistance is also related to charge behavior at interface, above changes suggest that interface states are behind such behavior with frequency [47,48]. High value of series resistance at low frequencies is due to an excess capacitance. Decrease in peak intensity indicates interface states non response to alternating current. Above 800 kHz, peak disappears completely. Peak intensity may be taken as a measure of active interface states density and carriers mobility.

5-Conclusion

Electrical properties of ZnO/SiC Schottky diodes with two SiC polytypes and two doping natures are investigated using I–V, C–V–f and Gp/

###

-V–f measurements. Parameters of interest are Schottky barrier height (###

*), ideality factor (n), series resistance (Rs), carriers concentrations (Nd, Na) and interface states*

_{b}density (Nss). Current through ZnO/n-4HSiC is higher than that through ZnO/n-6HSiC because of its

higher vertical a-axis electron mobility. Rectifying ratio (IF/IR), from ZnO/n-4HSiC is found to be twice that of ZnO/n-6HSiC. Devices exhibited very good rectification ratio, substantially low leakage current and indicate formation of excellent diodes between ZnO and n-type SiC with a noticeable superiority for 4HSiC substrates.

The small difference in barrier high from the J–V value between devices with different polytypes can be attributed to difference in band gap between 6H-SiC and 4H-SiC substrate which is about 3 eV and 3.2eV, respectively. Barrier height obtained from the C–V measurement is comparatively larger than barrier heights obtained from J–V measurements. Difference is attributed to interface effects. Barrier height is found to be around 0.9372 eV for ZnO/n-6HSiC and 1.1638 eV, For ZnO/n-4HSiC respectively. Interface states density was estimated to be 4.54*1011eV-1cm-2 for ZnO/n-6HSiC. Difference in barrier heights between ZnO/n-6HSiC and ZnO/n-4HSiC is about 0.22 eV, which corresponds to difference between their respective band gaps.

Series resistance determined from H(J) versus J plots are in good agreement with those obtained from dV/dLn(J) versus J plots. ZnO/n-6HSiC had a higher series resistance than ZnO/n-4HSiC devices. This can be attributed to carriers’ removal effect, mobility change and/or reduction in free carriers

‘concentrations.

Nss values for ZnO/n-6HSiC are lower than ZnO/n-4HSiC. Such behavior can be ascribed to a thicker

oxide layer at ZnO/n-6HSiC interface than at ZnO/n-4HSiC interface. This is due to a difference in interface dangling bonds between 6HSiC and 4HSiC surfaces.

## ACCEPTED MANUSCRIPT

Nss values for ZnO/p-4HSiC are lower than ZnO/n-4HSiC. Since interface states play a very important role in current flow mechanism in electronic devices, one may conclude that carrier’s recombination will be important in ZnO/n-4HSiC leading to I-V characteristics dominated by recombination.

Measured capacitance of Schottky diodes ZnO/ SiC changed with bias voltage and frequency. It is found that doping effect has lead to a 5 times higher peak for N type SiC than P type SiC, while a difference in polytypes has lead to a 2 times higher peak for 4HSiC than 6H SiC. These results reflect differences in interface states densities or traps densities between ZnO/n- 4H SiC, ZnO/p- 4H SiC and ZnO/n-6HSiC Schottky diodes.

One can see that conductance of Schottky diode ZnO/n-6HSiC, ZnO/n-4HSiC is very different from that of ZnO/p-4HSiC. As expected, conductance increases with increasing positive voltage for ZnO/n-type SiC and with increasing negative voltage for ZnO/p-type SiC. It decreases with increasing frequency in all cases due to increasing deactivation of interface states responsible for capture and emission of carriers. Series resistance changes with frequency for ZnO/ 6HSiC, ZnO/ n-4HSiC and ZnO/p-4HSiC Schottky diodes. For N type devices, series resistance peak decreases with higher frequencies and slightly shifts with greater voltages. Opposite behavior is seen to happen for P type devices. Since series resistance is also related to charge behavior at interface, above changes suggest that interface states are behind such behavior with frequency. High value of series resistance at low frequencies is due to an excess

## ACCEPTED MANUSCRIPT

Reference

[1] L. Boussouar, et al.,Investigation of barrier inhomogeneities in Mo/4H–SiC Schottky diodes,Microelectronic Engineering.6 (2011)969–975.

[2] W.Yu, Chun-Sheng .Wang, Wan-Bing .Lu, Shuang-Kui. Cui, Deposition of n-type nanocrystalline SiC films and current transport mechanisms in nanocrystalline SiC/crystalline Si heterojunction, Solid State Commun.143 (2007) 228 –231.

[3] Ü.Özgür, et al., A comprehensive review of ZnO materials and devices, J. Appl. Phys. 98 (2005). [4] Chennupati.Jagadish, Stephen J. Pearton, Zinc Oxide Bulk, Thin Films and Nanostructures, Elsevier. (2006).

[5] I. Hussain, M. Y. Soomro, N.Bano, O. Nur,M. Willander, Interface traps characterization and electrical proprieties of Au-ZnO nanorods Schottky diodes by conductance and capacitance methods, J. Appl. Phys. 112, 064506(2012).

[6] B.M. Ataev, Ya.I. Alivov, E.V. Kalinina, V.V. Mamedov, G.A. Onushkin, S. Sh. Makhmudov, A.K. Omaev, Heteroepitaxial ZnO/6H-SiC structures fabricated by chemical vapor deposition, J. Cryst. Growth 275(2005)2471–2474.

[7] Ya.I. Alivov, et al., Photoresponse of n-ZnO∕p-SiC heterojunction diodes grown by plasma-assisted molecular-beam epitaxy, Appl. Phys. Lett. 86 (2005).

[8] Ya.I. Alivov, et al., High efficiency n-ZnO/p-SiC heterostructures photodiodes grown by plasma-assisted molecular-beam epitaxy, Superlattices Microstruct. 38 (2005) 439–445.

[9] Yuen, et al., Control of conduction type in Al- and N-codoped ZnO thin films, Appl. Phys. Lett. 86 (2005).

[10] Y.T. Shih, et al., ZnO-based heterojunction light-emitting diodes on p-SiC(4H) grown by atomic layer deposition, Appl. Phys. B 98 (2010)767-772.

[11] J.F. Felix, E.F. da Silva Jr., E.A. de Vasconcelos, W.M. de Azevedo, Electrical and microscopic characterization of ZnO films on p-SiC substrates, Solid State Commun.151(2011) 1252-1255. [12] M. W. Allen, S. M. Durbin, J. B. Metson, Silver oxide Schottky contacts on nn-type ZnO, Appl. Phys. Lett. 91(2007).

[13] X. Zhang, F. Hai, T. Zhang, C. Jia, X. Sun, L. Ding, W. Zhang, Analysis of the electrical

characteristics of the Ag/ZnO Schottky barrier diodes on F-doped SnO2 glass substrates by pulsed laser deposition, Microelectron. Eng. (2012) 5–9.

[14] W. I. Park, G. C. Yi, J. W. Kim, S. M. Park, Schottky nanocontacts on ZnO nanorod arrays, Appl. Phys. Lett. 82(2003).

[15] Z. Y. Zhang, C. H. Jin, X. L. Liang, Q. Chen, L. M. Peng, Current-voltage characteristics and parameter retrieval of semiconducting nanowires, Appl. Phys. Lett. 88(2006).

[16] Rhoderick.E.H, R. H. Williams, Metal Semiconductor Contacts , Oxford University Press, (1988). [17] M. Biber, M. Cakar, A. Turut, The effect of anodic oxide treatment on n-GaAs Schottky barrier diodes, J. Mater. Sci.Mater. Electron. 12(2001)575 -579.

[18] H. Kim, H. Kim, D. W. Kim, Silver Schottky contacts to a-plane bulk ZnO, J. Appl. Phys.108(2010). [19] W.A. Hill, C.C. Coleman, A single-frequency approximation for interface-state density

determination, Solid-State Electron. 23 (1980) 987–993.

[20] M.R. Jennings, et al., Analysis of Al/Ti, Al/Ni multiple and triple layer contacts to p-type 4H-SiC, Solid-State Electron. 51 (2007)797–801.

[21] Shu-Cheng Chang, Shui-Jinn Wang, Kai-Ming Uang, Bor-Wen Liou, Investigation of Au/Ti/Al ohmic contact to N-type 4H-SiC. Solid-State Electron. 49(12) (2005)1937–1941.

[22] J. Johnson Brian, Michael A. Capano,Mechanism of Ohmic behavior of Al-Ti contacts to p type 4H-SiC after annealing, J.Appl.Phys.95(2004).

[23] Masaya.Kimura,Masashi.Kato,Masaya.Ichimura, Improvement of Schottky contact characteristics by anodic oxidation of 4H-SiC,Mater.Sci.Vol.679(2011)461-464.

[24] C. Temircl, B. Bati, M. Salam , A. Türüt, High-barrier height Sn/p-Si schottky diodes with interfacial layer by anodization process, Applied Surface Science,Vol. 172 (2001)1 –7.

[25] Simon. M. Sze, Kwok.K. Ng, Physics of Semiconductor Devices, John Wiley & Sons, (2006). [26] M.Asghar, K.Mahmood, M. Faisal1nd M. A Hasan, Electrical characterization of Au/ZnO/Si Schottky contact ,Journal of Physics,Conference Series 439 (2013) 012030.

## ACCEPTED MANUSCRIPT

[28] Dieter. K. Schroder, Semiconductor Material and Device Characterization, John Wiley & Sons, New York, (1998), pp. 168–205.

[29] H. Mathieu, Physique des semiconducteurs et des composants electroniques,fourth(ed.), Dunod, Paris, (2001).

[30] A. El-Shaer, A. Bakin, E. Schlenker et al., Fabrication and characterization of n-ZnO on p-SiC heterojunction diodes on 4H-SiC substrates, Superlattices and Microstructures, vol. 42 (2007)387–391. [31] Sze.Simon.M, Physics of Semiconductor Devices, 2nd edition,(1998).

[32] Xiangping. Li, Baolin. Zhang, Xin. Dong, Yuantao. Zhang, Xia. Xiaochuan, Wang. Zhao , Guotong. Du, Room temperature electroluminescence from ZnO/Si heterojunction devices grown by metal–organic chemical vapor deposition, J. Lumin. 129 (2009) 86-89.

[33] S.K. Cheung, N.W. Cheung, Extraction of Schottky diode parameters from forward current–voltage characteristics, Appl.Phys. Lett. (1986).

[34] M. W. Allen , S. M. Durbin, Inﬂuence of oxygen vacancies on Schottky contacts to ZnO, Appl.Phys. Lett, vol. 92 (2008).

[35] Şükrü.Karataş, Effect of series resistance on the electrical characteristics and interface state energy
distributions of Sn/*p*-Si (MS) Schottky diodes, Microelectronic Engineering. vol.87, no. 10, (2010)1935–
1940.

[36] A. Sertap.Kavasoglu, C. Tozlu, O. Pakma, Investigation of temperature dependent dc current
transport mechanism on Au/poly(4-vinyl phenol)/p-Si device, J. Phys. D, Appl. Phys. 42 (2009).
[37] A. Tataroğlu, Ş. Altındal, Analysis of interface states and series resistance of MIS Schottky diodes
using the current–voltage (*I*–*V*) characteristics, Microelectronic Engineering. Vol.85, no.1, (2008)233–
237.

[38] J. F. Felix, M. Aziz, W. M. de Azevedo,D. L. da Cunha,E. F. da Silva, Jr.,K. F. Seidel,D. Taylor,I. A. Hummelgen, M. Henin, investigation of deep-level defect in conductive polymer on n-type 4H- and 6H-sillicon carbide substrates using I-V and deep level transient spectroscopy techniques, J.App.Phys .112 (2012).

[39] R.T. Tung, Electron transport at metal–semiconductor interfaces, general theory, Phys. Rev. B 45 (1992).

[40] J.H. Werner, H.H. Guttler, Barrier inhomogeneities at Schottky contacts, J. Appl. Phys. 69 (1991)1522–1533.

[41] E.H. Nicollian, A. Goetzberger, The Si–SiO2 interface–electrical properties as determined by the metal–insulator conductance technique, Bell Syst. Tech. J. 46 (1967)1055 –1133.

[42] H. Kanbur, S. Altındal, A. Tataroglu, Appl. Surf. Sci. 252 (2005) 1732–1738.

[43] E.H. Nicollian, J.R. Brews, MOS (Metal/Oxide/Semiconductor) Physics and Technology, Wiley, New York, (1982).

[44] K.K. Hung, Y.C. Cheng, Characterization of Si–SiO2 interface traps in p-metal-oxide-semiconductor structures with thin oxides by conductance technique, J. Appl. Phys. 62 (1987).

[45] I. Dokme, S. Altındal, The C–V–f and G/w–V–f characteristics of Au/SiO2/n-Si capacitors,Physica B. 391 (2007) 59–64.

[46] Mehmet Cavasn, Analysis of interface states of GaAs-rhodamine hybrid diode by Hill–Coleman method, Volume 74 (2013) 892–895.

[47] Wadi.B.B,M.A.Kadaoui ,A.Saidane,M.Henini,M.Shafi,influence of annealing on electrical characteristics of Ti/Au/GaAsN Schottky diode with 0.2%

nitrogenincorporation,Material.Sci.Semiconductor.Processing.22(2014)92-100.

## ACCEPTED MANUSCRIPT

**Figure.1.**

### Schematic diagram of Ni/Al/SiC/ZnO heterojunction.

**Figure.2.**

### Current-voltage characteristics of investigated SiC-ZnO Schottky diodes.

**(a)**

### Effect of

### polytype structure.

**(b)**

### Effect of doping nature.

**Figure.3. **

### Logarithmic plots of J-V characteristics of ZnO-SiC.

** (a)**

### Effect of polytype structure.

**(b)**

### Effect of doping nature.

**Figure.4**

### . dV/dln (J) vs.J and H (J) vs. J plots of ZnO-SiC.

**(a)**

### Effect of polytype structure.

**(b)**

### Effect of doping nature.

**Figure.5.**

### Typical (1/C

2### –V) of ZnO-SiC.

**(a)**

### Effect of polytype structure.

**(b)**

### Effect of doping

### nature.

**Figure.6.**

### Forward capacitance–voltage-frequency characteristics for ZnO-SiC.

**(a)**

### ZnO/n-6HSiC,

**(b)**

### ZnO/n-4HSiC and

**(c)**

### ZnO/p-4HSiC.

**Figure.7**

### . G/ω–V characteristics of ZnO-SiC.(a)ZnO/n-6HSiC,

**(b)**

### ZnO/n-4HSiC and

**(c)**

### ZnO/p-4HSiC

**Figure.8.**

### Interface states density versus frequency for ZnO-SiC Schottky diodes.

**(a)**

### Effect of

### polytype structure.

**(b)**

### Effect of doping nature.

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

## ACCEPTED MANUSCRIPT

**Table 1**

### .Experimental barrier height (

###

_{b}### ), current saturation (Js), series resistance (Rs) and

### ideality factor (n) determined from I-V characteristics

## ACCEPTED MANUSCRIPT

Sample Carrier

concentration ND-NA (cm-3)

0
*b*

###

*(eV)*C-V ZnO/n-6HSiC ZnO/n-4HSiC 0.53956x10+15 0.50692x10+15 0.9372 1.1638

ZnO/p-4HSiC 23.4 x10+15 0.8230

Sample ideality

factor
(n)
*b*

###

*(eV)*(J-V) Rs dV/dLn(J)-J () Rs H(J)-J ()

Js(A/cm2) Current saturation ZnO/n-6HSiC ZnO/n-4HSiC 6.32 6.70 0.63 0.65 205.5 15.5 218.5 14.5 2.102x10-6 9.663x10-7